diffracting particle size analysis of martensite - retained austenite
Embed Size (px)
Transcript of diffracting particle size analysis of martensite - retained austenite
DIFFRACTING PARTICLE SIZE ANALYSIS OF MARTENSITE - RETAINED AUSTENITE MICROSTRUCTURES.
J. D. Makinson, W. N. Weins, T. W. Snyder, and R. J. De Angelis
Center for Materials Research and Analysis Department of Mechanical Engineering
University of Nebraska-Lincoln Lincoln, NE 68588
Case carburized steels containing a martensite-retained austenite microstructure are typically analyzed for the amount of each phase using x-ray diffraction techniques which are well established. In addition, however, analysis of the diffracting particle size of both the retained austenite and the martensite provides additional detailed information about the microstructure. The diffracting particle size of the martensite was measured as a function of depth of four end-quench specimens (Jominy bars) ranging from 0.22 to 0.83 weight percent carbon. In addition ,difFi-acting particle size of 53 case carburized samples was measured at a constant carbon composition, as a function of retained austenite content. Analysis of the data indicates that the diffracting particle size of the austenite becomes refined as the amount of martensite transforming from the austenite increases. This effect is due to the austenite being cut by the martensite and plastic deformation of the austenite by the martensite at lower temperatures. The martensite dX&actingparticle size remains relatively constant during transformation at a given carbon level, regardless of the degree of transformation. The martensite diffracting particle size does, however, increase as the morphology changes to a diffusion controlled transformation. I
Engineered components and structures which utilize steel as a material along with a quench and temper heat treatment will experience different cooling rates as a function of location during the quenching process. In addition, the product may have a variable carbon content as a function of location, due to processes such as carburization or decarburization of the surface of the component. The two phases which are most prevalent in this type of microstructures include martensite and retained austenite. While the amount of each phase is of great importance and is certainly the parameter which is most often measured using x-ray difiaction, the diffracting particle size of both the martensite and retained austenite as a function of carbon content and cooling rate are also of interest and can be determined at the same time generally using the same data. If the diffracting particle size can be correlated with the cooling rate and carbon content, it can be used as a method for checking the consistency of a particular heat treatment process, or to determine information about the processing parameters used for a particular heat treatment operation.
Copyright(c)JCPDS-International Centre for Diffraction Data 2000,Advances in X-ray Analysis,Vol.43 326ISSN 1097-0002
This document was presented at the Denver X-ray Conference (DXC) on Applications of X-ray Analysis. Sponsored by the International Centre for Diffraction Data (ICDD). This document is provided by ICDD in cooperation with the authors and presenters of the DXC for the express purpose of educating the scientific community. All copyrights for the document are retained by ICDD. Usage is restricted for the purposes of education and scientific research. DXC Website www.dxcicdd.com
ICDD Website - www.icdd.com
The specimens studied were standard Jominy bars machined from symmetrical positions of a single AISI-SAE 4320H grade steel bar, carburized, and then homogenized which resulted in carbon levels of 0.22,0.34,0.46, and.O.84%. Chemistry of the starting material is listed in Table 1. These four carbon levels were achieved by carburizing the specimens 0, 20, 40, and 120 hours respectively. Homogenization was carried out at 1200 C for 192 hours in a neutral atmosphere of argon. The grain size was then refined by two thermal cycling treatments after of the homogenization treatments Jere employed.
Element Weight %
Nickel 1.69% Manganese 0.61% ChOmiUm 0.57% Molybdenum 0.23% Silicon 0.30% Carbon 0.22% Phosphorous 0.021% Sulphur 0.020% Copper 0.14% Aluminum 0.05%
Table 1: Chemical analysis of the 4320H steel used for this investigation.
The Jominy bars were austenitized at 857C, held at temperature for 40 minutes, and then end-quenched as per ASTM A255. [I1 Water temperature was 16C. Flats were ground on the longitudinal sides of the Jominy bars and Rockwell hardness profiles were performed.
X-ray diffraction measurements were made by grinding to several depths from the quenched end of the four Jominy bars. Surface roughness after grinding measured less than 0.8 microns. The surface damaged layer was then removed by electropolishing at 25 to 35 volts for 120 seconds in a 6% perchloric, 35% buteoxyethanol, 59% methanol solution cooled by an ice water bath. This procedure removed eight to 16 pm of material. Finally, the electopolished surface was inspected using an optical microscope to ensure an uniform removal of material.
A Philips x-ray diffractometer was used with a copper anode tube powered at 40 kV and 30 mA. The diffractometer was outfitted with a graphite diffracted beam monochromator and a variable divergent slit. Since the cooling rate is a function of distance from the M(211) quenched end, copper k, radiation
was selected to minimize x-ray A(200) penetration depth. This decreased f _ I the range of cooling rates averaged
= into each x-ray measurement.
Higher carbon content in the steel increases the tetragonality of the as- quenched martensite unit cell. This
40 60 70 80 Two-Theta Degrees
is cka.dy seen in the x-ray p lgure 1: X-ray diffraction patterns of as-quenched diffraction pattern firom the as- 0.84% carbon steel.
Copyright(c)JCPDS-International Centre for Diffraction Data 2000,Advances in X-ray Analysis,Vol.43 327ISSN 1097-0002
quenched 0.84% carbon specimen in Figure 1. Because the amount of tetragonality depends on several factors such as carbon content and thermal history, the diffraction profile is affected to varying degrees. Although inexact, an assumption was made that the diftiaction profiles are symmetrical, therefore a method of reflecting the high angle side data to the low side was used, thus removing the asymmetric effect of the tetragonalality on the diffraction profile.
A single-profile Fourier analysis technique was used to determine the diffracting particle size L2]. This technique employs the Stokes correction for instrumental broadening. I31 Profiles from the NIST 660 LaB, standard reference material provide the instrument broadening function. The effective particle size was determined from the martensite M(200) reflection. Ferrous martensite contains very high dislocation densities in the order of 1Ol to 1012 per cm2. r41 With this heavy defect structure of the martensite, the x-ray line broadening is predominantly produced by small coherent particles.
Experimental Case Carburized Specimens
Fifty three 4320H steel specimens were case carburized with a 1 .O% carbon potential gas, cooled to room temperature then austenitized, followed by an oil quench. Finally, the specimens were tempered at 176C for three hours. The processing parameters such as austenitizing temperature, quench temperature, etc., were varied slightly to produce retained austenite contents ranging from 17 to 31%. Using a surface grinder, 500 pm of material was removed from the surface, then electropolished to remove the effects of grinding. Diffracting particle size was calculated from the retained austenite A(200) and martensite M(200) reflections. Because these specimens were tempered no teteragonality of the unit cell was present, therefore, it was not necessary to symmetrize the diffraction peak.
Retained austenite measurements were accomplished employing a four peak analysis method. The integrated intensities of two retained austenite, A(200) & A(220) and two martensite, M(200) & M(211) diffi-action peaks were used to calculate the retained austenite content. [51 These peaks are indexed and shown in Figure 1.
RESULTS AND DISCUSSION
Rockwell C hardness ofthe Jominy bars
0 60. = s Y 55. 8 @z 50. $3 g 45 - -E 2 40.
AAAAAAA *.AAA.AAA 00000000 AAAA
00 AA AA 0 AA
0 AA 0
0 OO AA 0.34 %C
ooooo 0.22 %C
0 10 20 30 40 50 Distance from Quenched End (mm)
as a function of distance from the Figure 2: Rockwell C hardness profile of the four end- quenched end are shown in Figure 2. quenched specimens. As expected, hardness increases with increasing carbon content. The lower carbon specimens exhibit decreased hardenability as compared to the higher carbon specimens. Both the 0.46% and 0.83% C specimens are through-hardened, maintaining their hardness 50 mm from the quenched end. Hardness of the 0.22 % C specimen
65 - l ********~~************* l ******* 0.83 %C
omo q OO~~OOOOOOO~OO~~OO~O~~~~OO 0.48 %C
Copyright(c)JCPDS-International Centre for Diffraction Data 2000,Advances in X-ray Analysis,Vol.43 328ISSN 1097-0002
begins to decrease at a depth 14 mm from the quenched surface, while the 0.34% C specimen begins to decrease at 25 mm.
The diffracting particle size of the martensite as a function of distance from the quenched end for all carbon levels are shown in Figure 3a. Figure 3b is enlarged area from Figure 3a. An overall decrease in diffracting particle si